acidity of twodimensional zeolites
Embed Size (px)
TRANSCRIPT
Acidity of twodimensional zeolitesThis journal is© the Owner
Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882 
27873
Cite this:Phys.Chem.Chem.Phys.,
Hybrid quantum mechanics:molecular mechanics (QM/MM) calculations of absolute deprotonation
energies are performed with periodic boundary conditions for Brønsted sites of aluminosilicate bilayers
with various Al/Si ratios (twodimensional zeolite). The supercell method is applied and density
functional theory is used. Much lower values are obtained (1042, 1069 and 1091 kJ mol1 for Al/Si = 1/63,
1/7 and 1/3, respectively) than those for bulk zeolites (1233 kJ mol1 for Hchabazite with Al/Si = 1/11).
We ascribe the much lower deprotonation energy to the smaller effective dielectric constant (1.6–1.9)
of an ultrathin dielectric in a vacuum compared to that of the corresponding bulk systems (3.0 for
Hchabazite), which leads to a better stabilization of the charge created upon deprotonation.
1. Introduction
Zeolites are crystalline porous aluminosilicates which are naturally occurring or synthesized. They are widely used as catalysts in industrial processes such as catalytic cracking of crude oil, methanol to gasoline conversion and olefin oligomerization.1,2
The catalytic activity of proton forms of zeolites originates from bridging Al–O(H)–Si groups which represent Brønsted acid sites.3,4
In recent years a particular class of materials, twodimensional zeolites, has attracted interest.5 They exist either as nanosheets, as thin as single unit cells of, e.g. MFI,6,7 or as ultrathin model systems grown under UHV conditions on metal substrates.8,9 The latter were prepared by the deposition of O2, Si and Al on the Ru(0001) surface and subsequent adsorption and desorption of water.8,9 They consist of an aluminosilicate bilayer with a twodimensional arrangement of hexagonal prisms and contain surface Brønsted sites.8 Thus, they may be considered as twodimensional zeolites (H2dH) with the flat surface corres ponding to the infinite pore size.9 The advantage of the H2dH thin films is that their properties can be analysed using surface science techniques.
Adsorption of the weak bases CO and C2H2 on the acidic site of the H2dH zeolite causes a red shift of the O–H stretching band that is considerably higher than the shift observed for the bulk HSSZ13 zeolite, the protonated form of Hchabazite (HCHA).8,9 This suggests that the twodimensional (2D) zeolite structures are considerably more acidic than the threedimensional (3D) ones.
The OH frequency shift upon adsorption of probe molecules10
is only one of the different measures of acidity strength.11–13 It is a reactivity parameter that assumes an ‘‘early’’ transition state. In contrast, adsorption of strong bases like ammonia or pyridine that have also been studied for H2dH and HCHA catalysts9
implies a late transition state with the proton being transferred to the reaction partner. However, the heat of ammonia adsorption depends on two factors, the intrinsic acidity of the Brønsted site (which is larger for the 2D zeolite) and the van der Waals interaction between the ammonium ion formed and the surface. The latter is larger for the curved surface of the porous material which is due to a better fit. A parameter that describes the intrinsic acidity without any interaction between the base molecule and the surface is the deprotonation energy (or the proton affinity of the deprotonated Brønsted site).4
The energy of adsorption, DEads, for the formation of an interacting ion pair
Z–OH + B  Z–OHB+ (1)
can be decomposed into the energy of the interaction, DEIP, between the protonated species and the deprotonated surface site,
Z–O + HB+  Z–OHB+ (2)
the deprotonation energy, DEDP, of the Brønsted site,
Z–OH  Z–O + H+ (3)
and the proton affinity, DEPA, of the base molecule
B + H+  HB+ (4)
Institut fur Chemie, HumboldtUniversitat zu Berlin, Unter den Linden 6,
10099 Berlin, Germany. Email: [email protected]
† Electronic supplementary information (ESI) available: Unit cell parameters, geometric parameters, figures of cluster models, and additional results for deprotonation energies as well as x, y, and z coordinates for selected structures. See DOI: 10.1039/c5cp05088j
Received 26th August 2015, Accepted 14th September 2015
DOI: 10.1039/c5cp05088j
27874  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
For molecules in the gas phase measuring the deprotonation energy (or the proton affinity) is a wellestablished technique. Mass spectrometry yields proton transfer equilibrium constants that are converted into gas phase acidity and gas phase basicity scales, e.g., ref. 14. For surface hydroxyl groups, however, quantum chemical calculations are the only source.4,11,15,16
The aim of this work is to determine the intrinsic acidity of H2dH zeolites by performing hybrid QM/MM calculations of the deprotonation energy, and to compare it with that of HCHA as an example of bulk zeolites. We also investigate the influence of the Al/Si ratio on the acidity of the H2dH system and we analyse the structure factors determining the deprotonation energies.
2. Methods 2.1 Periodicity and deprotonation energies
Zeolites are crystalline materials and theoretical investigations of their properties have to take into account the periodicity of the system. The deprotonation energy of a zeolite (DEDP) is defined as the energy difference between the deprotonated (Z–O) and the protonated (Z–OH) zeolite:
DEDP = EZO EZOH = DEv DP + Erel (6)
Using the energy of the deprotonated system ‘‘at the structure of’’ the parent system, EZO//ZOH, it may be decomposed into a ‘‘vertical’’ deprotonation energy, DEv
DP, and a relaxation energy, Erel,
Erel = EZO EZO//ZOH (7a)
DEv DP = EZO//ZOH EZOH (7b)
Applying periodic boundary conditions to the deprotonation process implies that a negative charge is created in every unit cell. This causes divergence of the electrostatic energy for the deprotonated system, ZO. It is also an unrealistic model because in the catalytic process we do not expect release of a proton in every unit cell at the same time. The divergence of the electrostatic energy can be eliminated by adding a uniform background charge to the deprotonated unit cell. The spurious interaction between the charged defects can be reduced using the supercell method or approximately eliminated using the method proposed by Leslie and Gillan (LG method).17
2.1.1 The supercell approach. This is the simplest, but computationally most demanding method. We build a series of supercells by multiplying the original unit cell N times in every direction and calculate the deprotonation energy for each supercell. We remove only one proton per supercell. This way, the distance between charged defects increases, and the artificial anion–anion interaction decreases. The deprotonation energy of the zeolite becomes a function of N. In the limit of infinitely large N, its value, DEN
DP, is interpreted as the deprotonation energy needed to remove the proton from an isolated Brønsted site. In the N N N supercell, the cubic
root of the supercell volume, ffiffiffiffi V3 p
, can be defined as the average distance between the charged defect and its nearest periodic
images, hri. The deprotonation energy of the system can be extrapolated using the following equation:
DEDPðNÞ ¼ DE1DP þ A
rh i þ B
rh i3 ¼ DE1DP þ Ecorr (8)
where DEDP(N) is the deprotonation energy for the N N N supercell, and A and B are fitting parameters. The 1/r and 1/r3
terms of the total correction, Ecorr, correspond to charge–charge and dipole–dipole interactions, respectively, and the para meters A and B reflect the screening properties of the material.
2.1.2 Aperiodic correction. The method proposed by Leslie and Gillan17 relies on the macroscopic approximation. It assumes that the difference between the energy per unit cell for the periodic defect and for the isolated defect is equal to the interaction of a periodic array of point charges, E, immersed in a dielectric medium with the dielectric constant e of the system without defects. Therefore, the deprotonation energy can be expressed as:
DELG DP ¼ DEDP
E eðLGÞ (9)
In practice, E is the energy of the point charge (usually H+) placed in the unit cell of the investigated system immersed in the compensating background charge, whereas e(LG) is 1/3 of the trace of the static dielectric tensor of the system. Comparison of eqn (8) and (9) shows that, if both correction methods are correct, the relationship:
E e ¼ A
rh i3 (10)
holds, from which we can calculate an effective dielectric constant eeff(SC) from given A and B parameters. The Leslie– Gillan approach is valid if the original unit cell is big enough to encapsulate the structural deformation induced by the charged defect and the dielectric constant of the material is isotropic. Both conditions are usually fulfilled for bulk zeolites, and the Leslie–Gillan method of aperiodic correction is the method of choice for these materials.
2.2 Embedded cluster QM/MM calculations
To calculate the deprotonation energy of zeolites, we used a mechanical embedding scheme,18,19 which partitions the system (S) into the inner region (I) and the outer region (O). The dangling bonds of the inner part are saturated with hydrogen link atoms, and the inner part together with the link atoms forms the cluster (C). The total energy E(S) and the forces 
Fa(S) acting on the atoms are obtained as follows:18,19
E(S) = EQM(C) + EMM(S) EMM(C) (11a) 
Fa(S) = 
Fa,QM(C) + 
Fa,MM(S) 
Fb(S) = 
To the quantum mechanical results for the cluster, EQM(C) and 


This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27875
the double counting of the contributions coming from atoms in the inner region and artificial contributions from link atoms. For an atom a of the inner region, all three terms contribute to the force acting on it. For an atom b of the outer region, the force is obtained from the force field alone. A link atom is not moved according to the force acting on it. It is instead fixed on the bond which it terminates.19,20
If we apply the QMPot embedding scheme (eqn (11a)) to calculate the zeolite deprotonation energy and introduce the notation CH, SH, C and S, for the cluster C and the total system S of the protonated and deprotonated form, respectively, we obtain:
DEDP = DEDP(QM) + DEDP(MM) (12a)
DEDP(MM) = EMM(S) EMM(C) [EMM(SH) EMM(CH)] (12c)
If the cluster is large enough, the structural distortion upon deprotonation decays within the cluster region and the DEDP(MM) term consists only of electrostatic interactions, i.e. longrange contributions DELR.18 Hence,
DEDP = DEDP(QM) + DELR (13)
Effectively, the deprotonation energy of the whole system is the sum of the deprotonation energy of a cluster calculated at the QM level and the longrange term representing the electrostatic interaction between the inner and the outer part of the system. This long range term is described at the MM level. Thus, the choice of an appropriate force field is crucial for the success of QM/MM calculations. To check if the applied embedding scheme works correctly, the convergence of the deprotonation energy with respect to the cluster size has to be investigated.
For the Leslie–Gillan method, with eqn (9) the total long range correction, DEN
LR, is given by
E eðLGÞ (14)
DEN
2.3 Details of QM/MM calculations
We used the QMPOT package,19,20 with DFT for the QM part and the DFTparametrized polarizable shell model potential of Sierka and Sauer21 for the MM part. The DFT calculations of energies and forces were done using the TURBOMOLE22
package with the B3LYP functional and the TZVP basis set named ‘‘def2’’ in the TURBOMOLE library.23,24 The latter includes the following contracted functions: H: (5s1p)/[3s1p], O: (11s6p2d1f)/[5s3p2d1f], and Si/Al: (14s9p3d1f)/[5s5p2d1f]. The choice of functional is based on previous experiences,21,25
and motivated by the fact that deprotonation energies of small aluminosilicate clusters calculated with the B3LYP functional
are in very good agreement with the CCSD(T) results (see Table S1 in the ESI†). For the shell model MM calculations, we used the GULP code,26 with parameters derived from B3LYP cluster calculations.21 It was shown21 that for this combination of QM and MM methods deprotonation energies of zeolites converge to a constant value with increasing cluster size. This indicates that the polarizable shellmodel force field describes the electro static interactions as accurately as the B3LYP functional.
3. Results 3.1 HCHA
The HCHA zeolite is chosen as a reference system because it consists of hexagonal prisms as secondary building units like the H2dH zeolite (Fig. 1).9 All tetrahedral atoms of HCHA are crystallographically equivalent (Fig. 1) and there are only four distinct oxygen positions.28 The energies of structures with the proton attached to different oxygen positions are similar,25
therefore we calculate deprotonation energies for the lowest energy structure only, i.e. with the proton attached to the O1 oxygen. We used a unit cell consisting of 37 atoms,20,21 with HAlSi11O24 composition and cell parameters optimised using the shell model potential (see Table S2 in the ESI†). These unit
Fig. 1 Optimized 2 2 2 unit cell of HCHA zeolite together with the numbering of oxygen atoms. The following colour scheme is adopted: silicon, oxygen, aluminium and hydrogen are depicted in yellow, red, grey and white, respectively. The pictures of molecular models were generated using the Jmol program.27
PCCP Paper
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
27876  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
cell parameters were fixed during subsequent structure optimi sation of protonated and deprotonated forms of the zeolite, for which we used the following convergence criteria: a maximum energy change of 1 105 eV, a maximum gradient component of 1 102 eV Å1, and a maximum displacement component of 1 103 Å. Cluster models of increasing size were generated automatically by selecting only those tetrahedral sites which were within a defined distance from the O1 site.
The QM clusters were always terminated with OH groups with a fixed OH distance of 96.1 pm (Fig. 2). This is an equilibrium distance that we obtained by free cluster optimization of similar cluster models.
To compare Leslie–Gillan deprotonation energies (eqn (9)) with those obtained using the supercell method we performed calculations for an embedded 8T12OH cluster model (eight tetrahedral sites terminated by 12 OH groups) with increasing supercell size from 2 2 2 to 4 4 4. Fig. 3 and Table 1 show that the corrected deprotonation energies of both methods, DE LG
DP and DE N
DP, agree within 0.6 kJ mol1. The increase of DEDP(QM/MM) with increasing cell size is
perfectly compensated by the decrease of the aperiodic correc tion, E/e(LG) (Leslie–Gillan method) or by the decrease of the A/hri, +B/hri3 correction term (supercell method) so that the DELG
DP and DEN
DP values, respectively, are perfectly converged already for the smallest 2 2 2 cell.
The dielectric constants calculated from the fitted para meters A and B (Fig. 3) and the average dielectric constants calculated for the LG correction method from the shellmodel
potential are virtually identical. The variation of e(LG) with the cell size is less than 2%, with the cluster size (Table 2) being slightly larger, 5%.
The QM part of the deprotonation energy is almost independent of the supercell size. This shows that the cluster structure is not affected by the unit cell size and structural distortions do not extend beyond the 2 2 2 supercell. In absolute terms, the
Fig. 2 Cluster models applied in QM/MM calculations of the HCHA deprotonation energy.
Fig. 3 Uncorrected deprotonation energies of the 8T12OH cluster model of HCHA embedded in N N N supercells (black dots). The solid line is the fitting curve, eqn (8). Deprotonation energies corrected using the LG method (red triangles) as a function of the cubic root of the unit cell volume and extrapolated deprotonation energy (dashed line).
Paper PCCP
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27877
charge–charge interaction, A/hri, is more than two orders of magnitude larger than the dipole–dipole aperiodic correction term, B/hri3 (Table 1). This supports the assumption of Leslie and Gillan that the aperiodic correction is given by the charge– charge interaction. We use the A/hri term only to correct all subsequent deprotonation energies of the HCHA zeolite.
The results obtained with embedded clusters of increasing size (Table 2) show that the corrected deprotonation energies of the HCHA zeolite converge to 1233 5 kJ mol1. This energy is in very good agreement with the value of 1231 kJ mol1, determined using the QM/MM methodology with a smaller basis set,29 and with the value of 1235 kJ mol1 obtained from the planewave DFT calculation with the BLYP functional (corrected for the systematic error of the functional).29 A periodic planewave DFT calculation with the PW91 functional yields a deprotonation energy of 1176 kJ mol1,30 but this value does not include the aperiodic correction and should be compared with our uncorrected value, 1164 kJ mol1. The remaining difference is small due to different basis sets and density functionals.
As we can see from Table 2, increasing the cluster size decreases the QM contribution of the deprotonation energy and simultaneously increases the total long range correction by almost the same value. This shows that the force field describes
the electrostatic interaction consistent with the (B3LYP) functional used for its parametrization. This has been documented before for Hartree–Fock calculations with correspondingly para metrized force fields.18 Geometric parameters of the acidic site are not strongly affected by the size of the QM region, and their values converge to constant values with increasing cluster size (see ESI,† Table S3). These all facts prove that the applied QM/MM methodology is appropriate to describe the properties of zeolites. Therefore, it can be used to predict the deprotonation energy of the H2dH system.
3.2 Ultrathin H2dH zeolite
To study the acidity of the ultrathin H2dH zeolite, we per formed calculations for cells of HnAlnSi64nO128 with increasing Al/Si ratio (Fig. 4), namely 1/63 (n = 1), 1/7 (n = 8) and 1/3 (n = 16). The cells for the different Al/Si ratio have the same size, but correspond to 1 1, 2 2, and 2 2 supercells, respectively, because the size of the primitive cells differs.
Experimentally, twodimensional zeolites were prepared on a Ru(0001) substrate.8,9,31 However the interaction between zeolite and the substrate was found to be weak31 and we excluded the ruthenium layer from our computational models. We applied 2D periodic boundary conditions and calculated electrostatic inter actions using the Perry summation technique,32,33 implemented in the GULP code.26 This was necessary because for standard slab calculations the energy of the charged system increases linearly with the vacuum thickness, and diverges in the limit of infinite values.34
First, we optimized the unit cell parameters using the shell model potential, which were kept fixed during all subsequent calculations. We prepared clusters of increasing size starting from a single hexagonal prism containing a Brønsted site (1D6R model) and adding up to 6 adjoining hexagonal prisms forming the 7D6R model (Fig. 5).
Table 1 Deprotonation energies (kJ mol1) and their components for the 8T12OH cluster model of HCHA embedded in different N N N supercells: DELG
DP and DEN
DP – deprotonation energies calculated using the Leslie–Gillan (LG) and supercell (SC) methods, respectively; DEDP(QM/
MM) and DEDP(QM) – (uncorrected) QM/MM deprotonation energy and its QM part, respectively. Dielectric constants calculated as 1/3 of the trace of the dielectric constant matrix at the MM level (shellmodel potential) (LG), and calculated from eqn (10) using the fitted parameters A and B, and eeff(SC)
Unit cell 2 2 2 3 3 3 4 4 4
DELG DP 1238.0 1238.0 1238.0
E/e(LG)a 37.6 24.9 18.6 DEDP(QM/MM) 1200.4 1213.1 1219.4 DEDP(QM) 1291.7 1292.4 1292.3 DEN
DP 1238.6 1238.6 1238.6 A/hrib 38.42 25.61 19.22 B/hri3 b 0.22 0.07 0.02 e(LG) 2.79 2.81 2.83 eeff(SC) 2.75 2.74 2.74
a Eqn (9). b Eqn (10).
Table 2 Deprotonation energy components (kJ mol1) for various embedded cluster models of the HCHA zeolite embedded in a 2 2 2 supercell. See Table 1 for definitions
Model DELG DP E/e(LG)a DEDP DEDP(QM) DEN
LR b e(LG)
MM 1036.4 34.0 1002.3 — — 3.09 8T12OH 1238.0 37.6 1200.4 1291.7 53.7 2.79 12T12OH 1239.3 36.1 1203.1 1276.4 37.1 2.91 16T16OH 1237.4 36.8 1200.7 1290.7 53.3 2.86 33T34OH
c 1233.5 24.7 1208.8 1267.3 33.8 2.83 44T34OH
c 1232.5 24.0 1208.5 1267.1 34.6 2.92
a Eqn (9). b Long range correction for LG corrected deprotonation energy, see eqn (13). c Cluster models embedded in a 3 3 3 supercell. Fig. 4 Optimized cells of the H2dH zeolite with different Al/Si ratios.
PCCP Paper
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
27878  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
In some cases it was necessary to add some extra tetrahedral sites to avoid terminal O–H groups that are connected to neighbouring Brønsted sites. These additional Tsites are indicated by a subscript, e.g. 4D6R+4T stands for four additional tetrahedral sites added to the 4DR6 cluster. Cluster models were terminated in the same way as for the HCHA zeolite.
The simple Leslie–Gillan method of aperiodic corrections is not applicable to the H2dH system. For the twodimensional case, the macroscopic approximation is not valid anymore. To calculate corrected deprotonation energies for the H2dH zeolites, we used the supercell extrapolation method which is computationally demanding. The original unit cells were multi plied in 
a and 
b directions and extrapolation curves, eqn (8), were fitted as a function of the square root of the surface area. A series of three supercells per each system, namely 1 1, 2 2, and 3 3 for Al/Si = 1/63, and 2 2, 3 3, and 4 4 for Al/Si = 1/7 and 1/3, were used to extrapolate deprotonation energies. All supercell structures were optimized, both the protonated and deprotonated forms. The resulting fitting parameters and correction energies are presented in the ESI,† Table S4 and Fig. S3.
For each Al/Si ratio the fitted parameters A and (especially) B depend on the cluster model. Nevertheless, the correction energies, Ecorr (eqn (8)), are almost constant within 6 kJ mol1. This means that one can calculate the aperiodic correction energy using the supercell approach for only one embedded cluster model, or even at the MM level, and then apply this correction for different embedded cluster models of the same unit cell, tolerating an error of about 6 kJ mol1.
The fitted A parameters are much larger for H2dH (ESI,† Table S4) than for HCHA (Fig. 3). This shows that in the two dimensional H2dH zeolite the interaction between charged defects is much less screened than that in the bulk HCHA zeolite. This is also reflected in very small effective dielectric constants of H2dH, 1.5–1.8 (Table 3), compared to 2.9–3.1 for HCHA (Table 2).
The extrapolated deprotonation energies of the H2dH zeolites converge to constant values with increasing embedded
cluster size (Table 3 and ESI,† Fig. S4), which is also true for the geometrical parameters of the Brønsted sites (see ESI,† Table S5). The deprotonation energies of all studied H2dH systems are much lower than those of HCHA. Even the least acidic two dimensional system with Al/Si = 1/3 has a deprotonation energy (1091 kJ mol1) which is 142 kJ mol1 lower than that of HCHA with Al/Si = 1/12.
Table 4 compares calculated deprotonation energies and their components for H2dH with different Al/Si ratios with those for HCHA. The table shows that the QM part of the deprotonation energy is significantly smaller for H2dH than that for HCHA. Nevertheless, the decisive factor for the very low deprotonation energy of twodimensional zeolites is the longrange term, which (in absolute terms) is a few times larger than that for HCHA.
The longrange component of the deprotonation energy results from the interactions between the inner part (cluster model) and its periodic surroundings. Upon removing the proton there is a change in the electrostatic (Coulomb and polarization) part of these interactions. The negative charge
Fig. 5 Cluster models applied in QM/MM calculations of the H2dH deprotonation energy (Al/Si = 1/63, models for the other Al/Si ratios are presented in Fig. S1 and S2 in the ESI†).
Table 3 Deprotonation energy components (kJ mol1) calculated for various embedded cluster models of H2dH zeolites for different Al/Si ratios using the supercell (SC) method
Al/Si Model DEN
DP DEQM DEN
LR Erel Ecorr(SC) eeff(SC)
1/63a MM 836.1 — — 184.3 44.3 1.529 1D6R 1032.1 1277.9 245.8 144.6 42.9 1.579 2D6R 1037.4 1244.7 208.5 139.9 42.9 1.579b
3D6R 1041.0 1232.6 182.0 143.2 45.3 1.493 4D6R 1041.5 1227.2 185.7 137.5 42.1 1.607 5D6R 1042.8 1217.6 174.9 137.3 42.1d 1.607d
6D6R 1044.8 1213.3 168.7 137.4 42.1d 1.607d
7D6R 1045.0 1210.1 165.1 136.9 42.1d 1.607d
1/7b MM 870.8 — — 191.3 42.5 1.591 1D6R+2T 1049.3 1320.4 271.2 142.5 37.9 1.781 2D6R+4T 1072.1 1249.2 177.1 137.2 44.3 1.523 3D6R+2T 1073.6 1238.3 164.7 137.8 44.3e 1.523e
4D6R 1068.9 1235.9 167.0 135.8 36.7 1.840 7D6R+4T 1071.8 1229.4 157.6 134.5 37.9 1.778
1/3c MM 890.3 — — 181.9 41.8 1.591 1D6R+4T 1069.6 1290.0 220.4 143.0 41.3 1.636 4D6R+4T 1090.6 1241.3 150.7 138.7 43.0 1.570
a 2 2 cell, hri = 39.9 Å. b 4 4 cell, hri = 40.0 Å. c 4 4 cell, hri = 40.2 Å. d Ecorr(SC), and eeff(SC) taken from the 4R6 model. e Ecorr(SC), and eeff(SC) taken from the 2R6 model.
Table 4 Calculated deprotonation energies and their components (kJ mol1) for twodimensional zeolites with different Al/Si ratios com pared to HCHA
Systema Model DEN
DP DEDP(QM) DEN
LR Erel eeff(SC)
HCHA (1/11) 44T32OH b 1233 1267 35 144 2.92
H2dH (1/63) 4D6Rc 1042 1227 186 138 1.61 H2dH (1/7) 4D6Rd 1069 1236 167 136 1.84 H2dH (1/3) 4D6R+4T
c 1091 1241 151 139 1.57
a Al/Si ratio is in parentheses. b 3 3 3 unit cell. c 2 2 unit cell. d 4 4 unit cell.
Paper PCCP
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27879
created upon deprotonation is stabilized by its surroundings. This stabilization is maximum if there is no screening of the created charge (e = 1). The more efficient the screening (the larger e), the smaller is the electrostatic stabilization of the created charge. For the H2dH zeolites the dielectric constant is relatively small, therefore the created charge is more stabilized by the crystal field than the one in HCHA. If this interpretation is correct, one should observe a dependence of the deprotonation energy of zeolites on their dielectric constant.
The geometric parameters of the Brønsted sites of H2dH (Al/Si = 1/63) and HCHA are almost the same (see ESI,† Tables S1 and S2) and the relaxation energies, Erel, of twodimensional and bulk zeolites (Table 4) are also very similar. Both these facts confirm that differences in long range electrostatic inter actions are indeed responsible for the observed differences in deprotonation energies.
3.3 Effect of the Al/Si ratio
The deprotonation energy of the H2dH zeolites increases with increasing Al/Si ratio (Table 4 and Fig. S4 in the ESI†). This behaviour was found in a number of experimental12,35,36
and theoretical studies.37–39 It suggests that an important factor governing the acidity of the Brønsted site is its local environment, i.e. the number of AlO4 tetrahedra in the second coordination sphere of the particular acidic site.12,35–38,40,41 An increase in the Al/Si ratio also affects the structure of the protonated and the deprotonated Brønsted sites (Table S5 in the ESI†), namely it decreases the Al–O bond length and the Al–O–Si angle and increases the Si–O bond length. Geometric parameters do not affect the relaxation energy of the anion, which is independent of the Al/Si ratio (Table 4). This suggests that the decrease of the acidity with increase of the Al content is caused mainly by the changes of the electronic structure of the zeolite. In 3D zeolites this effect is localised,37,38 namely it is caused by the interaction of the Brønsted site with its nearest surroundings. However, comparison of the QM and long range contributions of the deprotonation energies of H2dH zeolites (Table 4) shows that the increase of the Al/Si ratio also affects the long range term.
3.4 Dielectric screening in twodimensional systems
The small dielectric constant of the H2dH thin film can be explained by classical electrostatics, using the images.42
Let us first consider an electrostatic potential generated by a point charge q immersed in a homogeneous dielectric film, characterised by a dielectric constant e1 and the thickness L, surrounded by a medium with a dielectric constant e2 (Fig. 6 with e3 = e2).
The charge placed in the point (0, 0, a) generates the following potential (in atomic units) at the point (x, 0, a):43
V2D x; a;Lð Þ ¼ q
e1
g nj jffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi x2 þ L
g ¼ e1 e2ð Þ e1 þ e2ð Þ (16b)
an ¼ nLþ ð1Þn L
2 a
(16c)
Let us now consider an electrostatic potential generated by the point charge q immersed in the homogenous dielectric medium of a bulk system, characterized by the dielectric constant e. At a distance x from the charge the potential (in atomic units) is:
V3DðxÞ ¼ q
ex (17)
By comparison of eqn (16a) and (17) we can determine the effective dielectric constant eeff = e at the point (x, 0, a) of the dielectric slab:
eeff x; a;Lð Þ ¼ e1 x
Xn¼1 n¼1
g nj jffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi x2 þ L
1
(18)
In contrast to bulk dielectrics, the effective dielectric constant of thin layers depends on the distance from the charge (Fig. 7). Independent of the sample’s thickness, the effective dielectric constant on the surface (a = 0) changes continuously from (e1 + e2)/2 near the charge to e2 at an infinite distance from it (Fig. 7). In the case of the H2dH thin film, for which e1 (calculated as 1/3 of the trace of the dielectric constant tensor, which was determined from the shellmodel potential calculations) is about 5 and e2 is equal to 1 (vacuum), the theoretical dielectric constant should decrease from 3 near the charge to 1 at large distances. During derivation of eqn (18) a few assumptions were made, among others the assumption of homogenous dielectric medium and the assumption that the border between two dielectric media is sharp. Nevertheless, the calculated dielectric constant (1.6–1.9, Table 4) falls in the theoretical range (1 o eo 3), but a precise theoretical value cannot be specified.
We can use eqn (18) to predict the qualitative behaviour of zeolite dielectric properties. For example, we know that the effective dielectric constant depends on the distance a from the
Fig. 6 Model for dielectric constant calculations.
PCCP Paper
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
27880  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
surface (Fig. 7). In other words, when e1 4 e2, increasing a increases the dielectric constant. This is an important statement because it means that in the case of twodimensional zeolites we cannot compare uncorrected deprotonation energies of two different Brønsted sites which are at different distances from the surface, even though the size of the unit cell is the same. This also suggests that the acidity of the Brønsted sites which are deeper in the sample can be lower than of those which are at the surface. The thickness of the sample changes the slope of the dielectric constant curve, namely with decrease of L the curve becomes steeper (Fig. 7). Hence, we can expect that the acidity of the surface Brønsted sites should increase with decrease of the sample thickness. To confirm these predictions, a separate study of the thickness dependence of deprotonation energies for thin HMFI films6 is underway.
Let us consider the most general situation, namely a thin film characterized by a macroscopic dielectric constant e1
surrounded by different media at the top and the bottom with dielectric constants e2 and e3, respectively. This corresponds to our experimental model system, namely the ultrathin zeolite film deposited on the metal surface (e3 = N) under ultrahigh vacuum conditions (e2 = 1.0). Once again we can apply the macroscopic approximation to calculate the electrostatic potential
within a film and subsequently the effective dielectric constant of the film.43 Fig. 8 shows the effective dielectric constant within the thin layer as a function of a distance x from the point charge, calculated for different dielectric constants of the bottom layer. The effective dielectric constant on the slab surface (a = 0) changes continuously from (e1 + e2)/2 near the charge to (e2 + e3)/2 at large distances. It means that in the experimental case the dielectric screening near the charge is smaller than in the bulk zeolite, but for the bigger distances it quickly approaches infinity. Therefore the long range interaction between the active site and the crystal lattice should be much reduced with respect to the system without the metal substrate. If we assume that the influence of the metal substrate on the QM part of the deprotonation energy is not strong (short range interaction) we can expect that the acidity of the ultrathin zeolite adsorbed on the metallic surface should be reduced with respect to the freestanding film.
3.5 Comparison with OH frequency shifts
Since deprotonation energies cannot be directly measured for solid acids, a linear relationship has been suggested (Paukshtis and Yurchenko)44,45 between the OH frequency shift upon complex formation with a weak base molecule and the enthalpy of deprotonation, DHDP (kJ mol1):
DHDP = 1390 442.5log(D~nOH/D~nSiOH) (19)
Here, D~nOH and D~nSiOH are the wavenumber shifts for the O–H stretching vibrations of Brønsted sites and free silanols, respectively (in cm1), caused by the adsorption of weak bases. Because we are interested in the difference between two different zeolites, D(DEDP), we do not need to know D~nSiOH, which cancels out:
D(DEDP) E D(DHDP) = 442.5log(D~nOH(H2dH)/D~nOH(HCHA)) (20)
The wavenumber shifts upon CO adsorption from ref. 9, which have been calculated for exactly the same Si/Al = 7 bilayer as examined in the present study, yield a deprotonation energy
Fig. 7 Theoretical effective dielectric constant (eqn (18)) as a function of a distance x from the charge calculated for e1 = 5.0 and e2 = 1.0 and different a and L parameters.
Fig. 8 Theoretical effective dielectric constant as a function of a distance from the charge calculated for e1 = 5.0, e2 = 1.0, L = 5.3 Å, a = 0.0 Å and different dielectric constants of the bottom layer (e3).
Paper PCCP
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27881
difference of only 12 kJ mol1, one order of magnitude less than the calculated difference of 164 kJ mol1 from Table 4. Insertion of experimental values of D~nOH(H2dH) and D~nOH(HCHA), 379 and 316 cm1, respectively,9 into eqn (20) yields a larger deprotonation energy difference of 35 kJ mol1, but which is still much smaller than the calculated value of 164 kJ mol1.
The obvious reason for the breakdown of the DHDP D~nOH
plot is that the OH stretching frequency shift upon adsorption of CO refers to an ‘‘early’’ stage of the reaction, whereas deprotonation refers to a ‘‘late’’ stage of the catalytic reaction when the proton has been removed. This is consistent with the finding that the much larger acidity ‘‘measured’’ with the deprotonation energy is largely due to the better stabilization of the created negative charge in media with low dielectric constants such as twodimensional zeolites.
4. Conclusions
QM/MM calculations of deprotonation energies of ultrathin H2dH zeolites and the bulk HCHA zeolite confirm the much higher acidity of the ultrathin zeolites compared to bulk systems, previously observed in experiments.8,9 The very low deprotonation energy of the H2dH system reflects the fact that the dielectric constant of thin dielectrics immersed in a vacuum is much lower than that of corresponding bulk systems, resulting in a better stabilization of the charge created upon deprotonation. The dielectric constant of a thin film depends on its thickness and on the distance of the charge from the surface. This suggests that the properties of acidic sites in ultrathin zeolites6,7 and single layer zeolites8,9 vary with their distance from the surface and can be tuned by changing the sample’s thickness. Another consequence is that the acidity of twodimensional systems as judged upon deprotonation energies is much larger than OH frequency shifts upon adsorption of base molecules indicated.
Acknowledgements
This work has been supported by the German Research Foundation (DFG) through Collaborative Research Center Grant CRC 1109. The authors would like to thank Milan Oncak and Radosaw Wodarczyk for helpful discussions.
References
1 A. Corma, Chem. Rev., 1995, 95, 559. 2 A. Corma, J. Catal., 2003, 216, 298. 3 W. O. Haag, R. M. Lago and P. B. Weisz, Nature, 1984, 309, 589. 4 W. J. Mortier, J. Sauer, J. A. Lercher and H. Noller, J. Phys.
Chem., 1984, 88, 905. 5 W. J. Roth, P. Nachtigall, R. E. Morris and J. Cejka, Chem.
Rev., 2014, 114, 4807. 6 M. Choi, K. Na, J. Kim, Y. Sakamoto, O. Terasaki and
R. Ryoo, Nature, 2009, 461, 246. 7 Y. Seo, K. Cho, Y. Jung and R. Ryoo, ACS Catal., 2013, 3, 713.
8 J. A. Boscoboinik, X. Yu, B. Yang, F. D. Fischer, R. Wodarczyk, M. Sierka, S. Shaikhutdinov, J. Sauer and H.J. Freund, Angew. Chem., Int. Ed., 2012, 51, 6005.
9 J. A. Boscoboinik, X. Yu, E. Emmez, B. Yang, S. Shaikhutdinov, F. D. Fischer, J. Sauer and H.J. Freund, J. Phys. Chem. C, 2013, 117, 13547.
10 A. Zecchina, G. Spoto and S. Bordiga, Phys. Chem. Chem. Phys., 2005, 7, 1627.
11 J. Sauer, J. Mol. Catal., 1989, 54, 312. 12 W. E. Farneth and R. J. Gorte, Chem. Rev., 1995, 95, 615. 13 E. G. Derouane, J. C. Vedrine, R. R. Pinto, P. M. Borges,
L. Costa, M. A. N. D. A. Lemos, F. Lemos and F. R. Ribeiro, Catal. Rev., 2013, 55, 454.
14 J. E. Bartmess, J. A. Scott and R. T. McIver, Jr., J. Am. Chem. Soc., 1979, 101, 6046.
15 H. V. Brand, L. A. Curtiss and L. E. Iton, J. Phys. Chem., 1993, 97, 12773.
16 M. Brandle and J. Sauer, J. Am. Chem. Soc., 1998, 120, 1556. 17 M. Leslie and M. J. Gillan, J. Phys. C: Solid State Phys., 1985,
18, 973. 18 U. Eichler, M. Brandle and J. Sauer, J. Phys. Chem. B, 1997,
101, 10035. 19 U. Eichler, C. Kolmel and J. Sauer, J. Comput. Chem., 1997,
18, 463. 20 M. Sierka and J. Sauer, J. Chem. Phys., 2000, 112, 6983. 21 M. Sierka and J. Sauer, Faraday Discuss., 1997, 106, 41. 22 TURBOMOLE V6.4; a development of the University
of Karlsruhe and Forschungszentrum Karlsruhe GmbH, http://www.turbomole.com, 2012.
23 F. Weigend, M. Haser, H. Patzelt and R. Ahlrichs, Chem. Phys. Lett., 1998, 294, 143.
24 F. Weigend and R. Ahlrichs, Phys. Chem. Chem. Phys., 2005, 7, 3297.
25 M. Sierka and J. Sauer, J. Phys. Chem. B, 2001, 105, 1603. 26 J. D. Gale, J. Chem. Soc., Faraday Trans., 1997, 93, 629. 27 Jmol: an opensource Java viewer for chemical structures in
3D, http://www.jmol.org/. 28 M. Calligaris, G. Nardin, L. Randaccio and P. C. Chiaramonti,
Acta Crystallogr., 1982, 38, 602. 29 J. Sauer, K.P. Schroder and V. Termath, Collect. Czech.
Chem. Commun., 1998, 63, 1394. 30 C. Lo and B. L. Trout, J. Catal., 2004, 227, 77. 31 R. Wodarczyk, M. Sierka, J. Sauer, D. Loffler, J. J. Uhlrich,
X. Yu, B. Yang, I. M. N. Groot, S. Shaikhutdinov and H. J. Freund, Phys. Rev. B: Condens. Matter Mater. Phys., 2012, 85, 085403.
32 D. E. Parry, Surf. Sci., 1975, 49, 433. 33 D. E. Parry, Surf. Sci., 1976, 54, 195. 34 E. Wasserman, J. R. Rustad and A. R. Felmy, Surf. Sci., 1999,
424, 19. 35 H. Stach, J. Jaenchen, H. G. Jerschkewitz, U. Lohse, B. Parlitz
and M. Hunger, J. Phys. Chem., 1992, 96, 8480. 36 B. Gil, E. Broclawik, J. Datka and J. Klinowski, J. Phys. Chem.,
1994, 98, 930. 37 L. Grajciar, C. O. Arean, A. Pulido and P. Nachtigall, Phys.
Chem. Chem. Phys., 2010, 12, 1497.
PCCP Paper
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
27882  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
38 M. Sierka, U. Eichler, J. Datka and J. Sauer, J. Phys. Chem. B, 1998, 102, 6397.
39 A. G. Pel’menshchikov, E. A. Paukshtis, V. G. Stepanov, V. I. Pavlov, E. N. Yurchenko, K. G. Ione, G. M. Zhidomirov and S. Beran, J. Phys. Chem., 1989, 93, 6725.
40 G. M. Zhidomirov and V. B. Kazansky, in Advances in Catalysis, ed. D. D. Eley, H. Pines and P. B. Weisz, Academic Press, 1986, vol. 34, p. 131.
41 J. Datka and B. Gil, J. Catal., 1994, 145, 372. 42 J. Jackson, Classical Electrodynamics, Wiley, 3rd edn, 1998. 43 M. Kumagai and T. Takagahara, Phys. Rev. B: Condens.
Matter Mater. Phys., 1989, 40, 12359. 44 E. A. Paukshtis, R. I. Soltanov and E. N. Yurchenko, React.
Kinet. Catal. Lett., 1981, 16, 93. 45 A. P. Evgenii and E. N. Yurchenko, Russ. Chem. Rev., 1983,
52, 242.
Paper PCCP
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
Cite this:Phys.Chem.Chem.Phys.,
Hybrid quantum mechanics:molecular mechanics (QM/MM) calculations of absolute deprotonation
energies are performed with periodic boundary conditions for Brønsted sites of aluminosilicate bilayers
with various Al/Si ratios (twodimensional zeolite). The supercell method is applied and density
functional theory is used. Much lower values are obtained (1042, 1069 and 1091 kJ mol1 for Al/Si = 1/63,
1/7 and 1/3, respectively) than those for bulk zeolites (1233 kJ mol1 for Hchabazite with Al/Si = 1/11).
We ascribe the much lower deprotonation energy to the smaller effective dielectric constant (1.6–1.9)
of an ultrathin dielectric in a vacuum compared to that of the corresponding bulk systems (3.0 for
Hchabazite), which leads to a better stabilization of the charge created upon deprotonation.
1. Introduction
Zeolites are crystalline porous aluminosilicates which are naturally occurring or synthesized. They are widely used as catalysts in industrial processes such as catalytic cracking of crude oil, methanol to gasoline conversion and olefin oligomerization.1,2
The catalytic activity of proton forms of zeolites originates from bridging Al–O(H)–Si groups which represent Brønsted acid sites.3,4
In recent years a particular class of materials, twodimensional zeolites, has attracted interest.5 They exist either as nanosheets, as thin as single unit cells of, e.g. MFI,6,7 or as ultrathin model systems grown under UHV conditions on metal substrates.8,9 The latter were prepared by the deposition of O2, Si and Al on the Ru(0001) surface and subsequent adsorption and desorption of water.8,9 They consist of an aluminosilicate bilayer with a twodimensional arrangement of hexagonal prisms and contain surface Brønsted sites.8 Thus, they may be considered as twodimensional zeolites (H2dH) with the flat surface corres ponding to the infinite pore size.9 The advantage of the H2dH thin films is that their properties can be analysed using surface science techniques.
Adsorption of the weak bases CO and C2H2 on the acidic site of the H2dH zeolite causes a red shift of the O–H stretching band that is considerably higher than the shift observed for the bulk HSSZ13 zeolite, the protonated form of Hchabazite (HCHA).8,9 This suggests that the twodimensional (2D) zeolite structures are considerably more acidic than the threedimensional (3D) ones.
The OH frequency shift upon adsorption of probe molecules10
is only one of the different measures of acidity strength.11–13 It is a reactivity parameter that assumes an ‘‘early’’ transition state. In contrast, adsorption of strong bases like ammonia or pyridine that have also been studied for H2dH and HCHA catalysts9
implies a late transition state with the proton being transferred to the reaction partner. However, the heat of ammonia adsorption depends on two factors, the intrinsic acidity of the Brønsted site (which is larger for the 2D zeolite) and the van der Waals interaction between the ammonium ion formed and the surface. The latter is larger for the curved surface of the porous material which is due to a better fit. A parameter that describes the intrinsic acidity without any interaction between the base molecule and the surface is the deprotonation energy (or the proton affinity of the deprotonated Brønsted site).4
The energy of adsorption, DEads, for the formation of an interacting ion pair
Z–OH + B  Z–OHB+ (1)
can be decomposed into the energy of the interaction, DEIP, between the protonated species and the deprotonated surface site,
Z–O + HB+  Z–OHB+ (2)
the deprotonation energy, DEDP, of the Brønsted site,
Z–OH  Z–O + H+ (3)
and the proton affinity, DEPA, of the base molecule
B + H+  HB+ (4)
Institut fur Chemie, HumboldtUniversitat zu Berlin, Unter den Linden 6,
10099 Berlin, Germany. Email: [email protected]
† Electronic supplementary information (ESI) available: Unit cell parameters, geometric parameters, figures of cluster models, and additional results for deprotonation energies as well as x, y, and z coordinates for selected structures. See DOI: 10.1039/c5cp05088j
Received 26th August 2015, Accepted 14th September 2015
DOI: 10.1039/c5cp05088j
27874  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
For molecules in the gas phase measuring the deprotonation energy (or the proton affinity) is a wellestablished technique. Mass spectrometry yields proton transfer equilibrium constants that are converted into gas phase acidity and gas phase basicity scales, e.g., ref. 14. For surface hydroxyl groups, however, quantum chemical calculations are the only source.4,11,15,16
The aim of this work is to determine the intrinsic acidity of H2dH zeolites by performing hybrid QM/MM calculations of the deprotonation energy, and to compare it with that of HCHA as an example of bulk zeolites. We also investigate the influence of the Al/Si ratio on the acidity of the H2dH system and we analyse the structure factors determining the deprotonation energies.
2. Methods 2.1 Periodicity and deprotonation energies
Zeolites are crystalline materials and theoretical investigations of their properties have to take into account the periodicity of the system. The deprotonation energy of a zeolite (DEDP) is defined as the energy difference between the deprotonated (Z–O) and the protonated (Z–OH) zeolite:
DEDP = EZO EZOH = DEv DP + Erel (6)
Using the energy of the deprotonated system ‘‘at the structure of’’ the parent system, EZO//ZOH, it may be decomposed into a ‘‘vertical’’ deprotonation energy, DEv
DP, and a relaxation energy, Erel,
Erel = EZO EZO//ZOH (7a)
DEv DP = EZO//ZOH EZOH (7b)
Applying periodic boundary conditions to the deprotonation process implies that a negative charge is created in every unit cell. This causes divergence of the electrostatic energy for the deprotonated system, ZO. It is also an unrealistic model because in the catalytic process we do not expect release of a proton in every unit cell at the same time. The divergence of the electrostatic energy can be eliminated by adding a uniform background charge to the deprotonated unit cell. The spurious interaction between the charged defects can be reduced using the supercell method or approximately eliminated using the method proposed by Leslie and Gillan (LG method).17
2.1.1 The supercell approach. This is the simplest, but computationally most demanding method. We build a series of supercells by multiplying the original unit cell N times in every direction and calculate the deprotonation energy for each supercell. We remove only one proton per supercell. This way, the distance between charged defects increases, and the artificial anion–anion interaction decreases. The deprotonation energy of the zeolite becomes a function of N. In the limit of infinitely large N, its value, DEN
DP, is interpreted as the deprotonation energy needed to remove the proton from an isolated Brønsted site. In the N N N supercell, the cubic
root of the supercell volume, ffiffiffiffi V3 p
, can be defined as the average distance between the charged defect and its nearest periodic
images, hri. The deprotonation energy of the system can be extrapolated using the following equation:
DEDPðNÞ ¼ DE1DP þ A
rh i þ B
rh i3 ¼ DE1DP þ Ecorr (8)
where DEDP(N) is the deprotonation energy for the N N N supercell, and A and B are fitting parameters. The 1/r and 1/r3
terms of the total correction, Ecorr, correspond to charge–charge and dipole–dipole interactions, respectively, and the para meters A and B reflect the screening properties of the material.
2.1.2 Aperiodic correction. The method proposed by Leslie and Gillan17 relies on the macroscopic approximation. It assumes that the difference between the energy per unit cell for the periodic defect and for the isolated defect is equal to the interaction of a periodic array of point charges, E, immersed in a dielectric medium with the dielectric constant e of the system without defects. Therefore, the deprotonation energy can be expressed as:
DELG DP ¼ DEDP
E eðLGÞ (9)
In practice, E is the energy of the point charge (usually H+) placed in the unit cell of the investigated system immersed in the compensating background charge, whereas e(LG) is 1/3 of the trace of the static dielectric tensor of the system. Comparison of eqn (8) and (9) shows that, if both correction methods are correct, the relationship:
E e ¼ A
rh i3 (10)
holds, from which we can calculate an effective dielectric constant eeff(SC) from given A and B parameters. The Leslie– Gillan approach is valid if the original unit cell is big enough to encapsulate the structural deformation induced by the charged defect and the dielectric constant of the material is isotropic. Both conditions are usually fulfilled for bulk zeolites, and the Leslie–Gillan method of aperiodic correction is the method of choice for these materials.
2.2 Embedded cluster QM/MM calculations
To calculate the deprotonation energy of zeolites, we used a mechanical embedding scheme,18,19 which partitions the system (S) into the inner region (I) and the outer region (O). The dangling bonds of the inner part are saturated with hydrogen link atoms, and the inner part together with the link atoms forms the cluster (C). The total energy E(S) and the forces 
Fa(S) acting on the atoms are obtained as follows:18,19
E(S) = EQM(C) + EMM(S) EMM(C) (11a) 
Fa(S) = 
Fa,QM(C) + 
Fa,MM(S) 
Fb(S) = 
To the quantum mechanical results for the cluster, EQM(C) and 


This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27875
the double counting of the contributions coming from atoms in the inner region and artificial contributions from link atoms. For an atom a of the inner region, all three terms contribute to the force acting on it. For an atom b of the outer region, the force is obtained from the force field alone. A link atom is not moved according to the force acting on it. It is instead fixed on the bond which it terminates.19,20
If we apply the QMPot embedding scheme (eqn (11a)) to calculate the zeolite deprotonation energy and introduce the notation CH, SH, C and S, for the cluster C and the total system S of the protonated and deprotonated form, respectively, we obtain:
DEDP = DEDP(QM) + DEDP(MM) (12a)
DEDP(MM) = EMM(S) EMM(C) [EMM(SH) EMM(CH)] (12c)
If the cluster is large enough, the structural distortion upon deprotonation decays within the cluster region and the DEDP(MM) term consists only of electrostatic interactions, i.e. longrange contributions DELR.18 Hence,
DEDP = DEDP(QM) + DELR (13)
Effectively, the deprotonation energy of the whole system is the sum of the deprotonation energy of a cluster calculated at the QM level and the longrange term representing the electrostatic interaction between the inner and the outer part of the system. This long range term is described at the MM level. Thus, the choice of an appropriate force field is crucial for the success of QM/MM calculations. To check if the applied embedding scheme works correctly, the convergence of the deprotonation energy with respect to the cluster size has to be investigated.
For the Leslie–Gillan method, with eqn (9) the total long range correction, DEN
LR, is given by
E eðLGÞ (14)
DEN
2.3 Details of QM/MM calculations
We used the QMPOT package,19,20 with DFT for the QM part and the DFTparametrized polarizable shell model potential of Sierka and Sauer21 for the MM part. The DFT calculations of energies and forces were done using the TURBOMOLE22
package with the B3LYP functional and the TZVP basis set named ‘‘def2’’ in the TURBOMOLE library.23,24 The latter includes the following contracted functions: H: (5s1p)/[3s1p], O: (11s6p2d1f)/[5s3p2d1f], and Si/Al: (14s9p3d1f)/[5s5p2d1f]. The choice of functional is based on previous experiences,21,25
and motivated by the fact that deprotonation energies of small aluminosilicate clusters calculated with the B3LYP functional
are in very good agreement with the CCSD(T) results (see Table S1 in the ESI†). For the shell model MM calculations, we used the GULP code,26 with parameters derived from B3LYP cluster calculations.21 It was shown21 that for this combination of QM and MM methods deprotonation energies of zeolites converge to a constant value with increasing cluster size. This indicates that the polarizable shellmodel force field describes the electro static interactions as accurately as the B3LYP functional.
3. Results 3.1 HCHA
The HCHA zeolite is chosen as a reference system because it consists of hexagonal prisms as secondary building units like the H2dH zeolite (Fig. 1).9 All tetrahedral atoms of HCHA are crystallographically equivalent (Fig. 1) and there are only four distinct oxygen positions.28 The energies of structures with the proton attached to different oxygen positions are similar,25
therefore we calculate deprotonation energies for the lowest energy structure only, i.e. with the proton attached to the O1 oxygen. We used a unit cell consisting of 37 atoms,20,21 with HAlSi11O24 composition and cell parameters optimised using the shell model potential (see Table S2 in the ESI†). These unit
Fig. 1 Optimized 2 2 2 unit cell of HCHA zeolite together with the numbering of oxygen atoms. The following colour scheme is adopted: silicon, oxygen, aluminium and hydrogen are depicted in yellow, red, grey and white, respectively. The pictures of molecular models were generated using the Jmol program.27
PCCP Paper
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
27876  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
cell parameters were fixed during subsequent structure optimi sation of protonated and deprotonated forms of the zeolite, for which we used the following convergence criteria: a maximum energy change of 1 105 eV, a maximum gradient component of 1 102 eV Å1, and a maximum displacement component of 1 103 Å. Cluster models of increasing size were generated automatically by selecting only those tetrahedral sites which were within a defined distance from the O1 site.
The QM clusters were always terminated with OH groups with a fixed OH distance of 96.1 pm (Fig. 2). This is an equilibrium distance that we obtained by free cluster optimization of similar cluster models.
To compare Leslie–Gillan deprotonation energies (eqn (9)) with those obtained using the supercell method we performed calculations for an embedded 8T12OH cluster model (eight tetrahedral sites terminated by 12 OH groups) with increasing supercell size from 2 2 2 to 4 4 4. Fig. 3 and Table 1 show that the corrected deprotonation energies of both methods, DE LG
DP and DE N
DP, agree within 0.6 kJ mol1. The increase of DEDP(QM/MM) with increasing cell size is
perfectly compensated by the decrease of the aperiodic correc tion, E/e(LG) (Leslie–Gillan method) or by the decrease of the A/hri, +B/hri3 correction term (supercell method) so that the DELG
DP and DEN
DP values, respectively, are perfectly converged already for the smallest 2 2 2 cell.
The dielectric constants calculated from the fitted para meters A and B (Fig. 3) and the average dielectric constants calculated for the LG correction method from the shellmodel
potential are virtually identical. The variation of e(LG) with the cell size is less than 2%, with the cluster size (Table 2) being slightly larger, 5%.
The QM part of the deprotonation energy is almost independent of the supercell size. This shows that the cluster structure is not affected by the unit cell size and structural distortions do not extend beyond the 2 2 2 supercell. In absolute terms, the
Fig. 2 Cluster models applied in QM/MM calculations of the HCHA deprotonation energy.
Fig. 3 Uncorrected deprotonation energies of the 8T12OH cluster model of HCHA embedded in N N N supercells (black dots). The solid line is the fitting curve, eqn (8). Deprotonation energies corrected using the LG method (red triangles) as a function of the cubic root of the unit cell volume and extrapolated deprotonation energy (dashed line).
Paper PCCP
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27877
charge–charge interaction, A/hri, is more than two orders of magnitude larger than the dipole–dipole aperiodic correction term, B/hri3 (Table 1). This supports the assumption of Leslie and Gillan that the aperiodic correction is given by the charge– charge interaction. We use the A/hri term only to correct all subsequent deprotonation energies of the HCHA zeolite.
The results obtained with embedded clusters of increasing size (Table 2) show that the corrected deprotonation energies of the HCHA zeolite converge to 1233 5 kJ mol1. This energy is in very good agreement with the value of 1231 kJ mol1, determined using the QM/MM methodology with a smaller basis set,29 and with the value of 1235 kJ mol1 obtained from the planewave DFT calculation with the BLYP functional (corrected for the systematic error of the functional).29 A periodic planewave DFT calculation with the PW91 functional yields a deprotonation energy of 1176 kJ mol1,30 but this value does not include the aperiodic correction and should be compared with our uncorrected value, 1164 kJ mol1. The remaining difference is small due to different basis sets and density functionals.
As we can see from Table 2, increasing the cluster size decreases the QM contribution of the deprotonation energy and simultaneously increases the total long range correction by almost the same value. This shows that the force field describes
the electrostatic interaction consistent with the (B3LYP) functional used for its parametrization. This has been documented before for Hartree–Fock calculations with correspondingly para metrized force fields.18 Geometric parameters of the acidic site are not strongly affected by the size of the QM region, and their values converge to constant values with increasing cluster size (see ESI,† Table S3). These all facts prove that the applied QM/MM methodology is appropriate to describe the properties of zeolites. Therefore, it can be used to predict the deprotonation energy of the H2dH system.
3.2 Ultrathin H2dH zeolite
To study the acidity of the ultrathin H2dH zeolite, we per formed calculations for cells of HnAlnSi64nO128 with increasing Al/Si ratio (Fig. 4), namely 1/63 (n = 1), 1/7 (n = 8) and 1/3 (n = 16). The cells for the different Al/Si ratio have the same size, but correspond to 1 1, 2 2, and 2 2 supercells, respectively, because the size of the primitive cells differs.
Experimentally, twodimensional zeolites were prepared on a Ru(0001) substrate.8,9,31 However the interaction between zeolite and the substrate was found to be weak31 and we excluded the ruthenium layer from our computational models. We applied 2D periodic boundary conditions and calculated electrostatic inter actions using the Perry summation technique,32,33 implemented in the GULP code.26 This was necessary because for standard slab calculations the energy of the charged system increases linearly with the vacuum thickness, and diverges in the limit of infinite values.34
First, we optimized the unit cell parameters using the shell model potential, which were kept fixed during all subsequent calculations. We prepared clusters of increasing size starting from a single hexagonal prism containing a Brønsted site (1D6R model) and adding up to 6 adjoining hexagonal prisms forming the 7D6R model (Fig. 5).
Table 1 Deprotonation energies (kJ mol1) and their components for the 8T12OH cluster model of HCHA embedded in different N N N supercells: DELG
DP and DEN
DP – deprotonation energies calculated using the Leslie–Gillan (LG) and supercell (SC) methods, respectively; DEDP(QM/
MM) and DEDP(QM) – (uncorrected) QM/MM deprotonation energy and its QM part, respectively. Dielectric constants calculated as 1/3 of the trace of the dielectric constant matrix at the MM level (shellmodel potential) (LG), and calculated from eqn (10) using the fitted parameters A and B, and eeff(SC)
Unit cell 2 2 2 3 3 3 4 4 4
DELG DP 1238.0 1238.0 1238.0
E/e(LG)a 37.6 24.9 18.6 DEDP(QM/MM) 1200.4 1213.1 1219.4 DEDP(QM) 1291.7 1292.4 1292.3 DEN
DP 1238.6 1238.6 1238.6 A/hrib 38.42 25.61 19.22 B/hri3 b 0.22 0.07 0.02 e(LG) 2.79 2.81 2.83 eeff(SC) 2.75 2.74 2.74
a Eqn (9). b Eqn (10).
Table 2 Deprotonation energy components (kJ mol1) for various embedded cluster models of the HCHA zeolite embedded in a 2 2 2 supercell. See Table 1 for definitions
Model DELG DP E/e(LG)a DEDP DEDP(QM) DEN
LR b e(LG)
MM 1036.4 34.0 1002.3 — — 3.09 8T12OH 1238.0 37.6 1200.4 1291.7 53.7 2.79 12T12OH 1239.3 36.1 1203.1 1276.4 37.1 2.91 16T16OH 1237.4 36.8 1200.7 1290.7 53.3 2.86 33T34OH
c 1233.5 24.7 1208.8 1267.3 33.8 2.83 44T34OH
c 1232.5 24.0 1208.5 1267.1 34.6 2.92
a Eqn (9). b Long range correction for LG corrected deprotonation energy, see eqn (13). c Cluster models embedded in a 3 3 3 supercell. Fig. 4 Optimized cells of the H2dH zeolite with different Al/Si ratios.
PCCP Paper
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
27878  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
In some cases it was necessary to add some extra tetrahedral sites to avoid terminal O–H groups that are connected to neighbouring Brønsted sites. These additional Tsites are indicated by a subscript, e.g. 4D6R+4T stands for four additional tetrahedral sites added to the 4DR6 cluster. Cluster models were terminated in the same way as for the HCHA zeolite.
The simple Leslie–Gillan method of aperiodic corrections is not applicable to the H2dH system. For the twodimensional case, the macroscopic approximation is not valid anymore. To calculate corrected deprotonation energies for the H2dH zeolites, we used the supercell extrapolation method which is computationally demanding. The original unit cells were multi plied in 
a and 
b directions and extrapolation curves, eqn (8), were fitted as a function of the square root of the surface area. A series of three supercells per each system, namely 1 1, 2 2, and 3 3 for Al/Si = 1/63, and 2 2, 3 3, and 4 4 for Al/Si = 1/7 and 1/3, were used to extrapolate deprotonation energies. All supercell structures were optimized, both the protonated and deprotonated forms. The resulting fitting parameters and correction energies are presented in the ESI,† Table S4 and Fig. S3.
For each Al/Si ratio the fitted parameters A and (especially) B depend on the cluster model. Nevertheless, the correction energies, Ecorr (eqn (8)), are almost constant within 6 kJ mol1. This means that one can calculate the aperiodic correction energy using the supercell approach for only one embedded cluster model, or even at the MM level, and then apply this correction for different embedded cluster models of the same unit cell, tolerating an error of about 6 kJ mol1.
The fitted A parameters are much larger for H2dH (ESI,† Table S4) than for HCHA (Fig. 3). This shows that in the two dimensional H2dH zeolite the interaction between charged defects is much less screened than that in the bulk HCHA zeolite. This is also reflected in very small effective dielectric constants of H2dH, 1.5–1.8 (Table 3), compared to 2.9–3.1 for HCHA (Table 2).
The extrapolated deprotonation energies of the H2dH zeolites converge to constant values with increasing embedded
cluster size (Table 3 and ESI,† Fig. S4), which is also true for the geometrical parameters of the Brønsted sites (see ESI,† Table S5). The deprotonation energies of all studied H2dH systems are much lower than those of HCHA. Even the least acidic two dimensional system with Al/Si = 1/3 has a deprotonation energy (1091 kJ mol1) which is 142 kJ mol1 lower than that of HCHA with Al/Si = 1/12.
Table 4 compares calculated deprotonation energies and their components for H2dH with different Al/Si ratios with those for HCHA. The table shows that the QM part of the deprotonation energy is significantly smaller for H2dH than that for HCHA. Nevertheless, the decisive factor for the very low deprotonation energy of twodimensional zeolites is the longrange term, which (in absolute terms) is a few times larger than that for HCHA.
The longrange component of the deprotonation energy results from the interactions between the inner part (cluster model) and its periodic surroundings. Upon removing the proton there is a change in the electrostatic (Coulomb and polarization) part of these interactions. The negative charge
Fig. 5 Cluster models applied in QM/MM calculations of the H2dH deprotonation energy (Al/Si = 1/63, models for the other Al/Si ratios are presented in Fig. S1 and S2 in the ESI†).
Table 3 Deprotonation energy components (kJ mol1) calculated for various embedded cluster models of H2dH zeolites for different Al/Si ratios using the supercell (SC) method
Al/Si Model DEN
DP DEQM DEN
LR Erel Ecorr(SC) eeff(SC)
1/63a MM 836.1 — — 184.3 44.3 1.529 1D6R 1032.1 1277.9 245.8 144.6 42.9 1.579 2D6R 1037.4 1244.7 208.5 139.9 42.9 1.579b
3D6R 1041.0 1232.6 182.0 143.2 45.3 1.493 4D6R 1041.5 1227.2 185.7 137.5 42.1 1.607 5D6R 1042.8 1217.6 174.9 137.3 42.1d 1.607d
6D6R 1044.8 1213.3 168.7 137.4 42.1d 1.607d
7D6R 1045.0 1210.1 165.1 136.9 42.1d 1.607d
1/7b MM 870.8 — — 191.3 42.5 1.591 1D6R+2T 1049.3 1320.4 271.2 142.5 37.9 1.781 2D6R+4T 1072.1 1249.2 177.1 137.2 44.3 1.523 3D6R+2T 1073.6 1238.3 164.7 137.8 44.3e 1.523e
4D6R 1068.9 1235.9 167.0 135.8 36.7 1.840 7D6R+4T 1071.8 1229.4 157.6 134.5 37.9 1.778
1/3c MM 890.3 — — 181.9 41.8 1.591 1D6R+4T 1069.6 1290.0 220.4 143.0 41.3 1.636 4D6R+4T 1090.6 1241.3 150.7 138.7 43.0 1.570
a 2 2 cell, hri = 39.9 Å. b 4 4 cell, hri = 40.0 Å. c 4 4 cell, hri = 40.2 Å. d Ecorr(SC), and eeff(SC) taken from the 4R6 model. e Ecorr(SC), and eeff(SC) taken from the 2R6 model.
Table 4 Calculated deprotonation energies and their components (kJ mol1) for twodimensional zeolites with different Al/Si ratios com pared to HCHA
Systema Model DEN
DP DEDP(QM) DEN
LR Erel eeff(SC)
HCHA (1/11) 44T32OH b 1233 1267 35 144 2.92
H2dH (1/63) 4D6Rc 1042 1227 186 138 1.61 H2dH (1/7) 4D6Rd 1069 1236 167 136 1.84 H2dH (1/3) 4D6R+4T
c 1091 1241 151 139 1.57
a Al/Si ratio is in parentheses. b 3 3 3 unit cell. c 2 2 unit cell. d 4 4 unit cell.
Paper PCCP
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27879
created upon deprotonation is stabilized by its surroundings. This stabilization is maximum if there is no screening of the created charge (e = 1). The more efficient the screening (the larger e), the smaller is the electrostatic stabilization of the created charge. For the H2dH zeolites the dielectric constant is relatively small, therefore the created charge is more stabilized by the crystal field than the one in HCHA. If this interpretation is correct, one should observe a dependence of the deprotonation energy of zeolites on their dielectric constant.
The geometric parameters of the Brønsted sites of H2dH (Al/Si = 1/63) and HCHA are almost the same (see ESI,† Tables S1 and S2) and the relaxation energies, Erel, of twodimensional and bulk zeolites (Table 4) are also very similar. Both these facts confirm that differences in long range electrostatic inter actions are indeed responsible for the observed differences in deprotonation energies.
3.3 Effect of the Al/Si ratio
The deprotonation energy of the H2dH zeolites increases with increasing Al/Si ratio (Table 4 and Fig. S4 in the ESI†). This behaviour was found in a number of experimental12,35,36
and theoretical studies.37–39 It suggests that an important factor governing the acidity of the Brønsted site is its local environment, i.e. the number of AlO4 tetrahedra in the second coordination sphere of the particular acidic site.12,35–38,40,41 An increase in the Al/Si ratio also affects the structure of the protonated and the deprotonated Brønsted sites (Table S5 in the ESI†), namely it decreases the Al–O bond length and the Al–O–Si angle and increases the Si–O bond length. Geometric parameters do not affect the relaxation energy of the anion, which is independent of the Al/Si ratio (Table 4). This suggests that the decrease of the acidity with increase of the Al content is caused mainly by the changes of the electronic structure of the zeolite. In 3D zeolites this effect is localised,37,38 namely it is caused by the interaction of the Brønsted site with its nearest surroundings. However, comparison of the QM and long range contributions of the deprotonation energies of H2dH zeolites (Table 4) shows that the increase of the Al/Si ratio also affects the long range term.
3.4 Dielectric screening in twodimensional systems
The small dielectric constant of the H2dH thin film can be explained by classical electrostatics, using the images.42
Let us first consider an electrostatic potential generated by a point charge q immersed in a homogeneous dielectric film, characterised by a dielectric constant e1 and the thickness L, surrounded by a medium with a dielectric constant e2 (Fig. 6 with e3 = e2).
The charge placed in the point (0, 0, a) generates the following potential (in atomic units) at the point (x, 0, a):43
V2D x; a;Lð Þ ¼ q
e1
g nj jffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi x2 þ L
g ¼ e1 e2ð Þ e1 þ e2ð Þ (16b)
an ¼ nLþ ð1Þn L
2 a
(16c)
Let us now consider an electrostatic potential generated by the point charge q immersed in the homogenous dielectric medium of a bulk system, characterized by the dielectric constant e. At a distance x from the charge the potential (in atomic units) is:
V3DðxÞ ¼ q
ex (17)
By comparison of eqn (16a) and (17) we can determine the effective dielectric constant eeff = e at the point (x, 0, a) of the dielectric slab:
eeff x; a;Lð Þ ¼ e1 x
Xn¼1 n¼1
g nj jffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi x2 þ L
1
(18)
In contrast to bulk dielectrics, the effective dielectric constant of thin layers depends on the distance from the charge (Fig. 7). Independent of the sample’s thickness, the effective dielectric constant on the surface (a = 0) changes continuously from (e1 + e2)/2 near the charge to e2 at an infinite distance from it (Fig. 7). In the case of the H2dH thin film, for which e1 (calculated as 1/3 of the trace of the dielectric constant tensor, which was determined from the shellmodel potential calculations) is about 5 and e2 is equal to 1 (vacuum), the theoretical dielectric constant should decrease from 3 near the charge to 1 at large distances. During derivation of eqn (18) a few assumptions were made, among others the assumption of homogenous dielectric medium and the assumption that the border between two dielectric media is sharp. Nevertheless, the calculated dielectric constant (1.6–1.9, Table 4) falls in the theoretical range (1 o eo 3), but a precise theoretical value cannot be specified.
We can use eqn (18) to predict the qualitative behaviour of zeolite dielectric properties. For example, we know that the effective dielectric constant depends on the distance a from the
Fig. 6 Model for dielectric constant calculations.
PCCP Paper
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
27880  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
surface (Fig. 7). In other words, when e1 4 e2, increasing a increases the dielectric constant. This is an important statement because it means that in the case of twodimensional zeolites we cannot compare uncorrected deprotonation energies of two different Brønsted sites which are at different distances from the surface, even though the size of the unit cell is the same. This also suggests that the acidity of the Brønsted sites which are deeper in the sample can be lower than of those which are at the surface. The thickness of the sample changes the slope of the dielectric constant curve, namely with decrease of L the curve becomes steeper (Fig. 7). Hence, we can expect that the acidity of the surface Brønsted sites should increase with decrease of the sample thickness. To confirm these predictions, a separate study of the thickness dependence of deprotonation energies for thin HMFI films6 is underway.
Let us consider the most general situation, namely a thin film characterized by a macroscopic dielectric constant e1
surrounded by different media at the top and the bottom with dielectric constants e2 and e3, respectively. This corresponds to our experimental model system, namely the ultrathin zeolite film deposited on the metal surface (e3 = N) under ultrahigh vacuum conditions (e2 = 1.0). Once again we can apply the macroscopic approximation to calculate the electrostatic potential
within a film and subsequently the effective dielectric constant of the film.43 Fig. 8 shows the effective dielectric constant within the thin layer as a function of a distance x from the point charge, calculated for different dielectric constants of the bottom layer. The effective dielectric constant on the slab surface (a = 0) changes continuously from (e1 + e2)/2 near the charge to (e2 + e3)/2 at large distances. It means that in the experimental case the dielectric screening near the charge is smaller than in the bulk zeolite, but for the bigger distances it quickly approaches infinity. Therefore the long range interaction between the active site and the crystal lattice should be much reduced with respect to the system without the metal substrate. If we assume that the influence of the metal substrate on the QM part of the deprotonation energy is not strong (short range interaction) we can expect that the acidity of the ultrathin zeolite adsorbed on the metallic surface should be reduced with respect to the freestanding film.
3.5 Comparison with OH frequency shifts
Since deprotonation energies cannot be directly measured for solid acids, a linear relationship has been suggested (Paukshtis and Yurchenko)44,45 between the OH frequency shift upon complex formation with a weak base molecule and the enthalpy of deprotonation, DHDP (kJ mol1):
DHDP = 1390 442.5log(D~nOH/D~nSiOH) (19)
Here, D~nOH and D~nSiOH are the wavenumber shifts for the O–H stretching vibrations of Brønsted sites and free silanols, respectively (in cm1), caused by the adsorption of weak bases. Because we are interested in the difference between two different zeolites, D(DEDP), we do not need to know D~nSiOH, which cancels out:
D(DEDP) E D(DHDP) = 442.5log(D~nOH(H2dH)/D~nOH(HCHA)) (20)
The wavenumber shifts upon CO adsorption from ref. 9, which have been calculated for exactly the same Si/Al = 7 bilayer as examined in the present study, yield a deprotonation energy
Fig. 7 Theoretical effective dielectric constant (eqn (18)) as a function of a distance x from the charge calculated for e1 = 5.0 and e2 = 1.0 and different a and L parameters.
Fig. 8 Theoretical effective dielectric constant as a function of a distance from the charge calculated for e1 = 5.0, e2 = 1.0, L = 5.3 Å, a = 0.0 Å and different dielectric constants of the bottom layer (e3).
Paper PCCP
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27881
difference of only 12 kJ mol1, one order of magnitude less than the calculated difference of 164 kJ mol1 from Table 4. Insertion of experimental values of D~nOH(H2dH) and D~nOH(HCHA), 379 and 316 cm1, respectively,9 into eqn (20) yields a larger deprotonation energy difference of 35 kJ mol1, but which is still much smaller than the calculated value of 164 kJ mol1.
The obvious reason for the breakdown of the DHDP D~nOH
plot is that the OH stretching frequency shift upon adsorption of CO refers to an ‘‘early’’ stage of the reaction, whereas deprotonation refers to a ‘‘late’’ stage of the catalytic reaction when the proton has been removed. This is consistent with the finding that the much larger acidity ‘‘measured’’ with the deprotonation energy is largely due to the better stabilization of the created negative charge in media with low dielectric constants such as twodimensional zeolites.
4. Conclusions
QM/MM calculations of deprotonation energies of ultrathin H2dH zeolites and the bulk HCHA zeolite confirm the much higher acidity of the ultrathin zeolites compared to bulk systems, previously observed in experiments.8,9 The very low deprotonation energy of the H2dH system reflects the fact that the dielectric constant of thin dielectrics immersed in a vacuum is much lower than that of corresponding bulk systems, resulting in a better stabilization of the charge created upon deprotonation. The dielectric constant of a thin film depends on its thickness and on the distance of the charge from the surface. This suggests that the properties of acidic sites in ultrathin zeolites6,7 and single layer zeolites8,9 vary with their distance from the surface and can be tuned by changing the sample’s thickness. Another consequence is that the acidity of twodimensional systems as judged upon deprotonation energies is much larger than OH frequency shifts upon adsorption of base molecules indicated.
Acknowledgements
This work has been supported by the German Research Foundation (DFG) through Collaborative Research Center Grant CRC 1109. The authors would like to thank Milan Oncak and Radosaw Wodarczyk for helpful discussions.
References
1 A. Corma, Chem. Rev., 1995, 95, 559. 2 A. Corma, J. Catal., 2003, 216, 298. 3 W. O. Haag, R. M. Lago and P. B. Weisz, Nature, 1984, 309, 589. 4 W. J. Mortier, J. Sauer, J. A. Lercher and H. Noller, J. Phys.
Chem., 1984, 88, 905. 5 W. J. Roth, P. Nachtigall, R. E. Morris and J. Cejka, Chem.
Rev., 2014, 114, 4807. 6 M. Choi, K. Na, J. Kim, Y. Sakamoto, O. Terasaki and
R. Ryoo, Nature, 2009, 461, 246. 7 Y. Seo, K. Cho, Y. Jung and R. Ryoo, ACS Catal., 2013, 3, 713.
8 J. A. Boscoboinik, X. Yu, B. Yang, F. D. Fischer, R. Wodarczyk, M. Sierka, S. Shaikhutdinov, J. Sauer and H.J. Freund, Angew. Chem., Int. Ed., 2012, 51, 6005.
9 J. A. Boscoboinik, X. Yu, E. Emmez, B. Yang, S. Shaikhutdinov, F. D. Fischer, J. Sauer and H.J. Freund, J. Phys. Chem. C, 2013, 117, 13547.
10 A. Zecchina, G. Spoto and S. Bordiga, Phys. Chem. Chem. Phys., 2005, 7, 1627.
11 J. Sauer, J. Mol. Catal., 1989, 54, 312. 12 W. E. Farneth and R. J. Gorte, Chem. Rev., 1995, 95, 615. 13 E. G. Derouane, J. C. Vedrine, R. R. Pinto, P. M. Borges,
L. Costa, M. A. N. D. A. Lemos, F. Lemos and F. R. Ribeiro, Catal. Rev., 2013, 55, 454.
14 J. E. Bartmess, J. A. Scott and R. T. McIver, Jr., J. Am. Chem. Soc., 1979, 101, 6046.
15 H. V. Brand, L. A. Curtiss and L. E. Iton, J. Phys. Chem., 1993, 97, 12773.
16 M. Brandle and J. Sauer, J. Am. Chem. Soc., 1998, 120, 1556. 17 M. Leslie and M. J. Gillan, J. Phys. C: Solid State Phys., 1985,
18, 973. 18 U. Eichler, M. Brandle and J. Sauer, J. Phys. Chem. B, 1997,
101, 10035. 19 U. Eichler, C. Kolmel and J. Sauer, J. Comput. Chem., 1997,
18, 463. 20 M. Sierka and J. Sauer, J. Chem. Phys., 2000, 112, 6983. 21 M. Sierka and J. Sauer, Faraday Discuss., 1997, 106, 41. 22 TURBOMOLE V6.4; a development of the University
of Karlsruhe and Forschungszentrum Karlsruhe GmbH, http://www.turbomole.com, 2012.
23 F. Weigend, M. Haser, H. Patzelt and R. Ahlrichs, Chem. Phys. Lett., 1998, 294, 143.
24 F. Weigend and R. Ahlrichs, Phys. Chem. Chem. Phys., 2005, 7, 3297.
25 M. Sierka and J. Sauer, J. Phys. Chem. B, 2001, 105, 1603. 26 J. D. Gale, J. Chem. Soc., Faraday Trans., 1997, 93, 629. 27 Jmol: an opensource Java viewer for chemical structures in
3D, http://www.jmol.org/. 28 M. Calligaris, G. Nardin, L. Randaccio and P. C. Chiaramonti,
Acta Crystallogr., 1982, 38, 602. 29 J. Sauer, K.P. Schroder and V. Termath, Collect. Czech.
Chem. Commun., 1998, 63, 1394. 30 C. Lo and B. L. Trout, J. Catal., 2004, 227, 77. 31 R. Wodarczyk, M. Sierka, J. Sauer, D. Loffler, J. J. Uhlrich,
X. Yu, B. Yang, I. M. N. Groot, S. Shaikhutdinov and H. J. Freund, Phys. Rev. B: Condens. Matter Mater. Phys., 2012, 85, 085403.
32 D. E. Parry, Surf. Sci., 1975, 49, 433. 33 D. E. Parry, Surf. Sci., 1976, 54, 195. 34 E. Wasserman, J. R. Rustad and A. R. Felmy, Surf. Sci., 1999,
424, 19. 35 H. Stach, J. Jaenchen, H. G. Jerschkewitz, U. Lohse, B. Parlitz
and M. Hunger, J. Phys. Chem., 1992, 96, 8480. 36 B. Gil, E. Broclawik, J. Datka and J. Klinowski, J. Phys. Chem.,
1994, 98, 930. 37 L. Grajciar, C. O. Arean, A. Pulido and P. Nachtigall, Phys.
Chem. Chem. Phys., 2010, 12, 1497.
PCCP Paper
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9:
27882  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
38 M. Sierka, U. Eichler, J. Datka and J. Sauer, J. Phys. Chem. B, 1998, 102, 6397.
39 A. G. Pel’menshchikov, E. A. Paukshtis, V. G. Stepanov, V. I. Pavlov, E. N. Yurchenko, K. G. Ione, G. M. Zhidomirov and S. Beran, J. Phys. Chem., 1989, 93, 6725.
40 G. M. Zhidomirov and V. B. Kazansky, in Advances in Catalysis, ed. D. D. Eley, H. Pines and P. B. Weisz, Academic Press, 1986, vol. 34, p. 131.
41 J. Datka and B. Gil, J. Catal., 1994, 145, 372. 42 J. Jackson, Classical Electrodynamics, Wiley, 3rd edn, 1998. 43 M. Kumagai and T. Takagahara, Phys. Rev. B: Condens.
Matter Mater. Phys., 1989, 40, 12359. 44 E. A. Paukshtis, R. I. Soltanov and E. N. Yurchenko, React.
Kinet. Catal. Lett., 1981, 16, 93. 45 A. P. Evgenii and E. N. Yurchenko, Russ. Chem. Rev., 1983,
52, 242.
Paper PCCP
O pe
n A
cc es
s A
rt ic
le . P
ub lis
he d
on 0
6 O
ct ob
er 2
01 5.
D ow
nl oa
de d
on 3
0/ 11
/2 01
5 10
:4 9: